Ⅰ Fabric Breaking Strength
Fabric breaking strength is also can be called tensile strength, which refers to the maximum tensile force when the specimen is stretched to break. It is one of the main standards to assess the intrinsic quality of textiles. The unit of fabric breaking strength is “Newton (N)” and it is used to evaluate the capability of the fabric to resist tensile damage.
Ⅱ Breaking Strength Testing
- Testing instruments and materials
Textile tensile testing machine（Picture 1）,a number of woven fabrics, fixtures, pre-tension, etc. .
Picture 1 Textile tensile testing machine
- Testing principles
A sample of a predetermined size is stretched at a constant elongation rate until it breaks, and record the breaking strength, elongation at break, etc.
- Testing methods
The common testing methods of breaking strength include reveled-strip method, grab method, shear strip method. (Picture 2) For the testing of woven fabrics, the reveled-strip method is used frequently. For some fabrics that can not or can not easily remove the edge, such as knitted fabrics, nonwoven fabrics, coated fabrics, etc., they can be tested by shear strip method. The width of the sample must be strictly controlled, otherwise it will greatly disturb the testing results.
(1) Prepare for the samples
- Plug in and turn on the switch, the screen shows the starting up notification. Press “F4 ” , the screen displays test screen. Start testing in this screen interface and check the testing data.
- Press the “function” key to enter the test method selection screen, press “Fl” and “F2 “to select the testing method (here you can choose the strip method to test). After selecting, press “confirm” key to enter the parameter setting screen; If the test method displaying on the interface currently is the method that you are going to choose, then without changing the test method, you can press the “set” key to enter the parameter setting screen directly.
- Move the cursor and input the relevant parameters. After completing, press the “confirm” key to enter the testing state screen. (Chart1）
- Select the required fixtures for the test and install it on the machine. The upper fixture should be installed below the sensor and connected to the sensor, and the lower fixture should be mounted on the pedestal.
- Move the stopper on the limit lever to the positioning hole corresponding to the test method and lock it to adjust the clamp distance.
- Set the speed of stretching and recovery. Press the “speed control” key to enter the speed setting screen, and input the corresponding parameters by pressing the “F2” “F3” key(“←” “→” key) and the number keys. Then press “F4” key (“confirm” key) to exit the speed setting screen.
Chart 1 The setting of the gauge length and tensile speed
|Gauge Length（mm）||Fabric Elongation at Break（%）||Tensile Speed(mm/min)|
- Press the “clear” key (the upper fixture should be without any external force).If the instrument has previous test data, press the “reset” key to clear all data.
- Put the sample strip into the fixture. Place one end of the sample into the clamp of the upper fixture on which the clamp is open and keep the sample vertical to the clamp and swivel the handle to clamp it. Put the other end of the sample into the lower fixture with a little force, and use pre-tension in the lower end of the sample to make the sample straight. The strength of the pre-tension is determined by the density of the sample. (Chart 2) Tighten the lower fixture and remove the pre-tension m
Chart 2 Pre-tension
|The Intensity of the Sample(g/㎡）||≦200||＞200,≦500||＞500|
- Press the “Start” button to test. The upper fixture moves upward until the sample strip breaks. If the test strip breaks within the clamp or clamping line, the test is invalid and need to retest.
- After the test, press “Fl” “F2″to check and record the data.